Metals 2012, 2, 329-343; doi:10.3390/met2030329
Application of Severe Plastic Deformation Techniques to
Magnesium for Enhanced Hydrogen Sorption Properties
Jacques Huot 1,*, Nataliya Ye. Skryabina 2 and Daniel Fruchart 3
1 Physics Department, Université du Québec à Trois-Rivières, 3351 des Forges, Trois-Rivières,
Québec, G9A 5H7, Canada
2 Department of Physics, Perm State University, 15, Bukirev street, 614990, Perm, Russia;
3 Institut Néel, 25 rue des Martyrs, BP 166, 38042 Grenoble Cedex 9, France;
* Author to whom correspondence should be addressed; E-Mail: email@example.com;
Tel.: +1-819-376-5011 (ext. 3576); Fax: +1-819-376-5164.
Received: 1 June 2012; in revised form: 14 August 2012 / Accepted: 15 August 2012 /
Published: 31 August 2012
Abstract: In this paper we review the latest developments in the use of severe plastic
deformation (SPD) techniques for enhancement of hydrogen sorption properties of
magnesium and magnesium alloys. Main focus will be on two techniques: Equal Channel
Angular Pressing (ECAP) and Cold Rolling (CR). After a brief description of these two
techniques we will discuss their effects on the texture and hydrogen sorption properties of
magnesium alloys. In particular, the effect of the processing temperature in ECAP on
texture will be demonstrated. We also show that ECAP and CR have produced different
textures. Despite the scarcity of experimental results, the investigations up to now indicate
that SPD techniques produce metal hydrides with enhanced hydrogen storage properties.
Keywords: magnesium; magnesium alloys; severe plastic deformations; ECAP;
Since the last few years the effects of mechanical deformation on the hydrogen storage behavior of
metal hydrides have been intensively studied. Mechanochemistry, mainly performed using Ball
Metals 2012, 2
Milling (BM), has demonstrated the possibility to conduct various reactions, such as synthesis of
nanocrystalline and amorphous materials at low temperatures without dissolution or fusion of the
reactants. Forty years after the pioneering works of Benjamin  the mechanochemical treatment of
substances in producing new thermodynamically stable and metastable materials, often non-achievable
by traditional methods, is well established and received industrial applications. While the method is
progressing at the industrial level, knowledge about the physical mechanisms operating during the
mechanochemical treatment (e.g., ball milling) is still very limited due to serious difficulties in
quantifying this complex process .
The mechanochemical techniques of ball-milling (BM) and severe plastic deformation (SPD)
methods are widely used in research laboratories as well as in the industry. In the field of metal
hydrides BM is intensively used for preparation of new compounds and to obtain nanocrystalline
structure. Mechanical milling effects could be enhanced by changing parameters such as milling
atmosphere (reactive milling), temperature, addition of anti-sticking agents, etc. This level of
sophistication led to impressive results in enhancement of hydrogen storage properties of metal hydrides
by the use of mechanical milling. The next challenge is to scale-up these types of technologies to
industrial levels. Here the main hurdle may be the high energy milling (power and time) which is most
usually needed for improving metal hydride properties. This imposes additional requirements in terms
of specific energy of the milling machine and size of batches that could be processed. These problems
are compounded if the milling has to be performed under hydrogen pressure and at high temperature.
One also has to take into account the safety aspect of handling metal hydrides. The engineering aspects
of these problems could surely be solved. The main challenge will be to keep the capital and operation
cost low in order to make the technology competitive. However, the use of this technique poses the
problem of scaling-up a high-energy density method.
In the case of SPD it has just recently been used for metal hydrides and the results are relatively
scarce. In an early investigation, Ueda et al. have prepared a Mg–Ni laminated composite by cold
rolling stacked Mg and Ni sheets . However, to obtain the intermetallic Mg2Ni the samples had to
be heat treated at 673 K. Similar results were later found by Pedneault et al. [4,5]. They showed that
cold rolling combined with heat treatment resulted in nanostructured metal hydrides with good
electrochemical properties. In the case of Ti-based alloys, Zhang et al. [5,6] studied the effect of cold
rolling on the hydrogen sorption properties of Ti–22Al–27Nb alloy and found better hydrogenation
kinetics for cold rolled samples but only for the first hydrogenation cycle. Magnesium alloys have
been studied by a few groups using different SPD techniques or combination of them [6–23]. These
studies will be discussed in more details in the next sections but the general conclusion is that SPD
techniques could improve the hydrogen sorption properties of magnesium alloys.
One important advantage of SPD techniques over high energy milling is that they are potentially
easier to scale up to industrial level. Therefore, the study of SPD applied to metal hydrides is
interesting from a fundamental point of view because of the different action of SPD on the processed
material compared to high energy milling and also from a practical point of view because of the
possibility of reducing cost of hydrides processing. In this paper we will review the use of two SPD
techniques, Equal Channel Angular Pressing (ECAP) and Cold Rolling (CR) for the preparation of
magnesium for hydrogen storage. After a short description of each technique we will present recent
studies of the use of them in the case of magnesium. More specific techniques such as High Pressure
Metals 2012, 2
Torsion (HPT) and Fast Forging (FF) are not considered here because at this moment very few
investigations have been realized.
2. Equal Channel Angular Pressing
2.1. Description of the Technique
In the Equal Channel Angular Pressing (ECAP) severe plastic deformations are introduced into a
material by forcing a sample (billet) with a piston through a die consisting of two channels of equal
cross-section, which intersect at an angle (Φ) between 90° and 120°  (see Figure 1). The outer arc
of curvature where the two channels intersect is labeled Ψ. Since the billet assumes the form and the
cross-section of the die, it can be repeatedly processed to increase the microstrain density and
simultaneously reduce the size of crystallites to meso- or nanometer down to 40 to 100 nm range.
ECAP is quite efficient in processing metals and allows to produce porosity-free materials in
substantial quantities with lower concentration of impurities and at a lower cost than ball-milling .
Through the crystallite size refinement process, the proportion of high angle grain boundary (HAGB)
increases due to dislocations recovery . High texturation effects could also be introduced by this
process, thus organizing specific grain boundaries distributions, indeed depending on the crystal
symmetry of the processed system (e.g., cubic versus hexagonal).
Figure 1. Schematic illustration of Equal Channel Angular Pressing (ECAP).
The equivalent strain (ε) introduced in the material by the ECAP process is determined by an
equation incorporating the angle between the two parts of the channel, Φ, and the angle representing
the outer arc of curvature where the two parts of the channel intersect, Ψ. The relationship given by: = 2 √3 cot Φ2 + Ψ2 +Ψ f N,Φ,Ψ (1)
Metals 2012, 2
where N is the number of passes through the die , and accounting the weakness of the f term
contribution an expression that is often simplified , to: = 1.15 cot Φ2 (2)
However, if the number of passes seems to be a dominant parameter, the most important refinement
of the microstructure takes place during the first pressing passes, since the development of an ultrafine
grain size leads to an increase of the yield stress.
2.3. Effect of Billet Rotation
From Figure 1 it could be seen that after a single pressing a cubic element is sheared into a
rhombohedral shape. If the same billet is pressed a second time then the operator has the choice to
insert the billet with or without rotation. It has been recognized that, for repetitive pressing, the overall
shearing characteristics within the crystalline sample may be changed by a rotation of the sample
between the individual pressings . When samples are pressed repetitively, different slip systems
may be introduced by rotating the samples about the X-axis between consecutive passes through the
die. Several processing routes have been identified for use in ECAP: route A in which the sample is
pressed repetitively without rotation, route BC in which the sample is rotated by 90° in the same sense
between each pass and route C where the sample is rotated by 180° between passes . More
complex combination of these routes could also be performed.
Inspection of Figure 2 shows that route A markedly increase the distortion of the rhombohedron,
route B increases the distortion in the X and Z planes and route C restores the cubic element so that
strain has been i